Composite Repair of ThroughWall Defects in Pipework  Analytical and Numerical Models with respect to ISO/TS 24817


 Evan Kelly
 2 years ago
 Views:
Transcription
1 Karlsruher Institut für Technologie Institut für Baustatik Composite Repair of ThroughWall Defects in Pipework  Analytical and Numerical Models with respect to ISO/TS 4817 M. Köpple, S. Lauterbach, W. Wagner Mitteilung (01) BAUSTATIK
2 Karlsruher Institut für Technologie Institut für Baustatik Composite Repair of ThroughWall Defects in Pipework  Analytical and Numerical Models with respect to ISO/TS 4817 M. Köpple, S. Lauterbach, W. Wagner Mitteilung (01) BAUSTATIK c Prof. Dr. Ing. W. Wagner Telefon: Institut für Baustatik Telefax: Karlsruher Institut für Technologie E mail: Kaiserstr. 1 Internet: Karlsruhe
3 Composite Repair of ThroughWall Defects in Pipework  Analytical and Numerical Models with respect to ISO/TS 4817 M.F. Köpple, S. Lauterbach, W. Wagner Karlsruhe Institute of Technology (KIT), Institute for Structural Analysis, Kaiserstr. 1, Karlsruhe, Germany Abstract A major problem for the oil and gas industry is the repair of corroded steel piping. As a replacement of affected sections usually results in high expenses for the operator, rehabilitation methods which can be implemented on an operating pipeline are favoured by the industry. The application of overwraps made of FibreReinforced Polymer systems offers such a promising method. In this work it is assumed that an overwrap is already installed, however, ongoing internal corrosion leads to a throughwall defect in the pipe. Hence, the fluid pressurises the repair and a detachment of the overwrap from the steel substrate can occur. This can even result in external leakage. In order to avoid this case of damage an analytical assessment approach is developed by means of Linear Elastic Fracture Mechanics and Finite Element Analysis. Subsequently, this approach is compared to the one given in the Code ISO/TS 4817 which is currently the mainly used code for the qualification and design of composite repairs for pipework. Keywords: Pipeline corrosion, FRP overwrap, Plate theory, Fracture mechanics, Finite element analysis (FEA) 1. Introduction The oil and gas industry uses steel pipelines as a basic element in the production and transport of oil and gas. Operating in harsh environmental conditions and transporting a wide range of highpressure fluids, pipelines can suffer from a variety of damage scenarios. These may include coating damage, erosion, corrosion or mechanical damage. One of the most common scenarios experienced by the industry is internal and/or external corrosion of the piping. Depending on the severity of the problem this can have significant detrimental effects on the pressure bearing capability of the pipelines and may lead to reduced life spans or at worst to a loss of structural integrity, i.e. failure. In order to extend the durability of pipelines, methods to repair such damage have been developed. A repair must be able to prevent leakage and also to restore all or part of the maximum allowable operating capacity of the pipeline. Usually, traditional repair methods require that the corroded or damaged piping is taken offline while the affected pipe section is replaced or reinforced by external steel strengthening/sealing elements. However, a plant shutdown imposes a significant loss in revenue on the operator. Consequently, rehabilitation methods which can be implemented without shutting down the production are favoured by the industry [1]. The use of FibreReinforced Polymer (FRP) systems for rehabilitation and retrofitting of deteriorating structural systems has been embraced worldwide. FRP materials are highly suited for use as repair material as they possess a very high specific strength and stiffness, a high formability and an inherent immunity to corrosion []. Hence, they have emerged in many industries over the past decades including aerospace, automotive, infrastructure and oil and gas. In the concrete and bridge industry, for instance, the loadcarrying capacity of reinforced concrete beams can be improved significantly by bonding FRP laminates to its tension flange [3, 4]. A recent application of FRPs for the oil and gas industry involves the repair of corroded pipelines by external wrapping of affected sections. Primary benefits associated with FRP overwrap repairs are a continuous fluid transmission while the repair is installed and the fact that no hot work or ignition is required and thus, the explosion potential is eliminated. This results in a significant improvement and reduction in repair costs [5, 6]. A major disadvantage in the use of FRP repairs is the complexity of possible failure mechanisms which can range from intralaminar failure (e.g. fibre fracture or fibrematrix debonding) to interlaminar failure, also known as delamination [7, 8]. If delamination occurs between two different materials, it is called bimaterial interface fracture. 1
4 In this paper fracture between a steel pipeline and an applied overwrap made of FRP is discussed. Therefore, it is assumed that ongoing internal corrosion leads to a relatively uniform loss of metal thickness and in extreme case to a throughwall defect in the pipeline. As a result the internal fluid pressure of the operating pipeline acts on the FRP/steel interface and a pressurised blister in the repair occurs. If the detachment of the repair from the pipeline propagates it results in external leakage. In order to ensure the applicability of FRP overwrap repair systems in case of internal corrosion, the processes of burst and leakage have to be investigated in detail. Previous work done by Mableson et al. [9] has shown that tubular pipe test samples and representative flat plate test samples, both composed of a steel substrate and a FRP repair, where blind holes were drilled into the steel, fail at very similar pressures. As a consequence, it is assumed that the effects of wall curvature can be neglected compared to the local stresses involved in the blister. And hence, flat plate models are regarded as a first approximation model to investigate delamination and blistering of an FRP overwrap repair system, respectively to deduce an analytical assessment approach which can be applied by the industry. This case of damage is considered in the code ISO/TS 4817 [10]. To assess the structural integrity of a FRP overwrap repair system, a theoretically based solution is provided to calculate the released energy in case of FRP/steel interface fracture. In this work an independent analytical fracture mechanics model is derived and subsequently compared to the ISOapproach. Further, several numerical investigations of the assumptions and accuracies implemented in the theoretically derived equations are discussed.. Theory Assuming that the adhesion between the steel substrate and the FRP repair is only given by brittle resin and that all work done in inflating the blister is stored as recoverable elastic strain energy, the principles of Linear Elastic Fracture Mechanics (LEFM) can be applied to investigate the behaviour of a pressurised blister formation. According to Griffth s fracture criterion [11, 1], fracture is only initiated if the energy release rate Γ is greater than or equal to the fracture toughness G c. In the case of linear elasticity it follows Γ = p dv da G c (1) where p is the applied pressure, and dv equals the change of blister volume during an infinitesimal crack advance da [13]. On the basis of Equation (1) two different scenarios can be considered. First, for laboratory testings, the crack resistance G c can be determined knowing the critical pressure of failure p crit and the material parameters, i.e. the applied repair thickness t and the elastic constants of Young s Modulus E, shear modulus G, and Poisson s ratio ν. The second scenario is the case of application. Knowing, the fracture toughness G c and the design pressure p, the required material parameter to avoid fracture can be determined by applying an upper limit of the occurring blister volume dv. However, both scenarios have in common that the function of the volume V, with V(E, G, ν, t), is known. Therefore, an analytical fracture mechanics model is developed in the following. 3. Analytical Analysis of Blister Formation Provided that the rotation of the crosssection of the repair is zero r = R, the behaviour of the pressurised repair is regarded to be equivalent to the one of a clamped circular plate, radius R, under uniform load p, as per Figure 1. Further, it is supposed that the FRP repair can be regarded as a quasiisotropic laminate, i.e. the inplane elastic constants are given by E = E 11 = E and ν = ν 1 = ν 1. The most significant modes of deformation that contribute to blister volume are assumed to be due to bending w b (r), transverse shear deformation w s (r) and local throughthickness compression w c(r). The first two modes refer to the rθz coordinate system which lies at the level of the repair midsurface, as per Figure 1. To consider the additional volumetric deflection due to throughthickness compression, the coordinate system rθz is introduced, with z = z t/, as per Figure 3. Assuming that the occurring deformations are small, the profile of the bending deflection component w b (r) for a clamped circular plate of radius R, carrying a uniformly distributed load p, is given after the Classical Plate Theory (CPT) [14] by w b (r) = p 64K (R r ) ()
5 Figure 1: Model of Pressurised Blister where K, known as flexural rigidity of the plate, is defined as K = Et 3 1(1 ν ) In case of the problem given, a high aspect ratio of repair thickness t to hole radius R, and a low transverse shear modulus G (= G 13 = G 3 ) compared to the inplane shear modulus G 1, can result in a large proportion of the total deflection w(r) associated with transverse shear. As the effects of transverse shear strains can often be neglected compared to those involved with bending, the case of a circular transverse elastic plate can be hardly found in literature. Therefore, an approach to determine the quantity of transverse shear deflection w s (r), based on the ideas of [14, 15] will be derived in detail in the upcoming paragraph. Considering the kinematics of a transverse elastic plate, as per Figure, it can be stated that the total plate rotation ψ r (r) is given by the straindisplacement relationship where [...], r refers to differentiation with respect to radius r and γ rz = ψ r + w, r (4) u r (z) = ψ r z (5) (3) Figure : Plate Kinematics The transverse shear stress τ rz, which has a parabolic distribution over the plate thickness, is given by τ rz (z) = Gγ rz = 3 ) t q r (1 4z With the use of Equation (5) and Equation (6), the horizontal deflection u r (z) can be calculated by integrating to τrz (z) u r (z) = G w, r dz = 3 ) Gt q r (z 4z3 zw, 3t r (7) 3 t (6)
6 where the boundary condition u r (0) = 0 was applied. Hence, the strain components ε r and ε θ for a rotationally symmetric plate are given by, see e.g. [15] ε r = u r, r = 3 ) Gt q r, r (z 4z3 zw, 3t rr ε θ = u r = 3 ) q r (z 4z3 zw, (8) r Gt r 3t r The resulting normal stresses σ r and σ θ are generally defined as, see e.g. [15] E σ r = 1 ν (ε r + νε θ ) E σ θ = 1 ν (νε r + ε θ ) and thus, the stresses σ r and σ θ due to the deflection u r (z) can be calculated to be ( E 3 4z3 σ r = (z 1 ν Gt 3t )(q r, r +ν q r z(w, rr +ν w, ) r ( E 3 4z3 σ θ = (z 1 ν Gt 3t )(νq r, r + q r z(νw, rr + w, ) (10) r Bending moments can be calculated by integrating plate stresses. Thus, the equations for a rotationally symmetric plate are given by m r = = m θ = = t/ t/ E 1 ν t/ t/ E 1 ν σ r z dz ( t 10G (q r, r +ν q r t3 1 (w, rr +ν w, ) r σ θ z dz ( t 10G (νq r, r + q r t3 1 (νw, rr + w, ) r Until this point no differentiation between bending w b (r) and shear deflection w s (r) was made. Therefore, the total deflection w(r) is replaced by the sum of w b (r) + w s (r) which leads m r = E ( t 1 ν 10G (q r, r +ν q r t3 1 (w s, rr +ν w ) s, r K(w b, rr +ν w b, r m θ = E ( t 1 ν 10G (νq r, r + q r t3 1 (νw s, rr + w ) s, r K(νw b, rr + w b, r It is stated that each second part of the above given equations equals the generally accepted expressions for the bending moments m r,b and m θ,b which can be derived for a transverse rigid plate, i.e. by neglecting the effects of transverse shear strains, see e.g. [14]. m r,b = K(w b, rr +ν w b, r m θ,b = K(νw b, rr + w (13) b, r 4 (9) (11) (1)
7 To assure that the total deflection w(r) can actually be separated into its single components w b (r) and w s (r), it is necessary that the bending moments m r,s and m θ,s due to shear drop out. As a consequence, the deflection w b (r) only results from bending and w s (r) from shear forces. It follows m r,s = m θ,s = E 1 ν E 1 ν ( t ) ) 10G (q r, r +ν q r t3 1 (w s, rr +ν w s, r ( t 10G (νq r, r + q r t3 1 (νw s, rr + w s, r The arising system of equations can be solved by equating the terms in parentheses which yields! = 0! = 0 (14) w s, r (r) = 6 5Gt q r (15) Applying equilibrium conditions it can be seen that the resultant of the applied load p is equal to the resultant of the reaction forces, which are defined positive in positive zdirection and hence, Equation (15) becomes q r = pr w s, r (r) = 3pr (17) 5Gt Finally, integrating and applying the edge condition w s (R) = 0 leads to an expression for the shear deflection w s (r): w s (r) = R 0 w s, r (r) dr = (16) 3p 10Gt (R r ) (18) It is supposed that, in addition to these components there will some further volumetric deflection due to local compression of the repair material under pressure. A first approximation to determine the quantity of this component can be made by comparing the occurring compression to the one around the upper half of a pennyshaped crack under internal pressure. This problem was originally considered by Sneddon [16] who calculated the conditions of rupture for an infinite solid containing a plane crack bounded by a circle. It was found that the crack, assumed to be originally an infinitely thin crevice, has, after the application of an internal pressure p, the shape of a very flat ellipsoid of revolution, where the vertical deflection is given by w c(r). A schemtical illustration of the undeformed and the deformed crack is shown in Figure 3. It is again noted that the coordinate system rθz is introduced, with z = z t/, to consider the deflection of the bottom edge of the repair. Figure 3: Undeformed and Deformed PennyShaped Crack With the use of equilibrium conditions for an axisymmetric volume element described by cylindrical coordinates, Harding and Sneddon [17] solved the arising system of equations by applying the following boundary conditions on the plane z = 0: (i) τ rz (r) = 0 for all values of r (ii) σ z (r) = p(r) for r < R 5
8 (iii) w c(r) = 0 for r > R Further, due to the rotational symmetry of the problem all derivatives with respect to θ are zero, as well as the stresses τ rθ = τ z θ = 0. Concerning the remaining stress components σ r, σ z, σ θ, τ rz it is noted that they have to tend to zero as r and/or z. If it is supposed that the applied pressure p(r) is constant over the entire crack surface 0 r R, the deflection component w c(r) is given by [16, 18] w c(r) = 4p(1 ν 13 ) πe 33 (R r ) 0.5 (19) It is obvious that the quantity of this component is determined by the transverse elastic constants E 33 and ν 13 to be applied in case of a quasiisotropic material. Finally, the volume of fluid in the pressurised blister due to bending (V b ), transverse shear (V s ) and throughthickness compression (V c ) is deduced from the sum of the three deflections by integrating: r=r V = π w(r)r dr r=0 r=r ( = π wb (r) + w s (r) + w c(r) ) r dr r=0 = πp(1 ν )R 6 16Et 3 } {{ } V b + 3πpR4 0Gt } {{ } V s + 8p(1 ν 13 )R3 3E 33 } {{ } V c (0) For convenience, an illustration of the occurring total blister volumes is given in Figure 4. Figure 4: Total Blister Volume The actual proportion of each volumetric deflection component of the total deflection is illustrated in Figure 5. The calculation is based on representative composite material parameters for a single ply, lamina, as given in Table 1, where the principles of the Classical Laminate Theory (CLT) were applied to determine the constants of a quasiisotropic laminate (QI), with [0, ±60 ] s [19]. The other parameter are given by p = 10 MPa, R = 10 mm and t = 5 mm. As already introduced above, the energy release rate Γ equals the change of potential energy dπ during an infinitesimally small crack advance da. In the case to be investigated the area of the crack is given by A = πr and thus, da = πr dr (1) Differentiating Equation (0) with respect to R and using Equation (1) to substitute da leads to an expression for the energy release rate Γ in case of a circular blister formation: Γ = p 3(1 ν ) R Et 3 0Gt R + (1 ν 13 ) R () E 33 π With Equation () an expression is deduced relating the energy release rate to the pressure, repair geometry and material properties. Substituting radius R by its diameter d/ and Γ by the fracture toughness G c, as well as considering 6
9 Parameter Lamina Laminate (QI) E 11 [GPa] E [GPa] E 33 [GPa] G 1 [GPa] G 13 [GPa].9.7 G 3 [GPa].6.7 ν 1 [ ] ν 13 [ ] ν 3 [ ] Table 1: Repair Material Parameter Deflection w(r) [mm] w b (r)+w s (r)+w c (r) w b (r)+w s (r) w b (r) Radius r [mm] Figure 5: Deflection Curves of Blister a number of n tests, where i = 1,,..., n, Equation () becomes p i = (1 ν ) E 3 51t 3 i G c,i d 4 i + (1 ν 13 ) E 33 1 π d i Gt i d i It is stated that under the initially made assumptions Equation (3) is very similar to the corresponding equation which can be found in the ISOCode [10] as follows p i = G c,i (1 ν ) 3 d 4 E ac 51ti 3 i + 1 π d i + 3 di 64Gt i However, a detailed comparison of both approaches highlights several differences. First, the ISOCode uses a combined tensile modulus E ac = E 11 E to consider a quasiisotropic material behaviour. This simplification is imprecise and not conform with the principles of the CLT. Further, it can be found that the used expression for transverse shear deflection in the ISOCode is overestimating the problem. It is supposed that it is based on the erroneous assumption that the shear stress τ rz (z) has a constant value of τ rz (0) = τ max over the plate thickness (cf. Equation (6)). Finally, if a deflection due to throughthickness compression shall be considered it is inevitable to use throughthickness Young s Modulus E 33 and Poission s ratio ν 13 for the corresponding compression term. This can yield significantly higher deflections than those obtained when the inplane constants E 11 (= E ) and ν 1 (= ν 1 ) are applied, as found in the ISOapproach. At this point it is generally stated that after Equation (1) an overestimation of volumetric deflection leads to an underestimation of the critical pressure of failure p crit and vice versa. 7 (3) (4)
10 4. Numerical Analysis of Blister Formation The analytical fracture mechanics model of a pressurised blister represents a first method to calculate the released energy in case of steel/frpinterface fracture. In order to assess the assumptions made in this approach, several numerical investigations based on Finite Element Analysis (FEA) are conducted. As discussed above the total volumetric deflection can be separated in three different modes bending, transverse shear and throughthickness compression. To prove the accuracy of each analytically derived term, a similar model geometry is required. Therefore, a clamped circular plate with radius R = 10 mm, thickness t =.5 mm (t = 5.0 mm) and load p = 10 MPa is modeled. The applied material properties are the same as the ones of the quasiisotropic laminate, as introduced in Table 1. Due to the rotational symmetry of the entire problem, including material properties, orthotropic axisymmetric ninenode solid elements are used [0]. To ensure that the occurring deformations are computed sufficiently precise, a number of 10 elements are used in throughthickness zdirection (0 elements for t = 5.0 mm). In radial rdirection the number of elements is 40. It is noted that due to symmetry conditions an equivalent modeling strategy could be the implementation of a threedimensional segment of a circle with an arbitrary opening angle. In terms of cylindrical coordinates, the indices 1,, 3 are replaced by r, θ, z. Accordingly, the stressstrain relations of an orthotropic axisymmetric solid element are given by, see e.g. [15] 1 ν rθ 0 ν rz E rr ε r ε θ γ rz ε z = E rr sym. E rr 1 0 ν θz E θθ E θθ 1 0 G rz As it can be seen from Equation (5) shear strains are generally not coupled to extensional loading in case of an orthotropic material. Hence, it is supposed that the portion of bending deflection w b (r) of the overall deflection w(r) can be extracted by a high increase of the transverse shear stiffness G rz (used factor = 100). To exclude additional deflection due to a compression and/or contraction of the plate, the load is divided in one half each on the bottom and the upper edge of the plate, and the deflection is analysed at the level of the midsurface. The analytical term for bending deflection w b (r) and the deflection curve achieved by FEA are illustrated in Figure 6 for both plate geometries. It can be seen that the curves show a high concordance. 1 E zz σ r σ θ τ rz σ z (5) Deflection w b (r) [mm] t/r = 0.50 t/r = 0.5 analytical numerical Radius r [mm] Figure 6: Bending Deflection (R = 10 mm) Since the CPT, which is basis for the analytical derivation of w b (r), basically requires a small ratio of t/r, it is obvious that the accuracy of the analytical approach declines with increasing ratio of t/r. To this effect, it could be shown that an adequate accuracy is only obtained for t/r 0.5, otherwise this component is overestimated. 8
11 As an extraction of pure shear deflection is not possible, the total deflection due to bending and shear is investigated. Applying the same model as before, but using the actual nonmodified material properties (cf. Table 1), it is found that the analytical and the numerical approach also yield similar deflection curves, as per Figure 7. Therefore, it is stated that the analytically derived term for transverse shear deflection w s (r) works accurately as well for t/r Deflection w b (r) + w s (r) [mm] t/r = 0.50 t/r = 0.5 analytical numerical Radius r [mm] Figure 7: Bending and Transverse Shear Deflection (R = 10 mm) In order to investigate the effect of an additional volumetric deflection due to throughthickness compression, the load p is fully applied on the bottom edge of the plate. Provided that neither bending nor shear deflection vary over the plate thickness, the quantity of compression can be estimated by calculating the difference in deflection of the bottom edge and the midsurface. To this effect, it is found that the percentage increase in deformation at r = 0 is vanishingly small for t = 5 mm (t/r = 0.5), but already amounts to 39% for t = 10 mm (t/r = 1.0), indicating that the influence of compression increases with increasing ratio t/r. Accordingly, Figure 8 shows a comparison between the calculated deflection curves due to throughthickness compression obtained by FEA and the analytical solution w c(r) after [16] Deflection w c (r) [mm] t/r = 8.0 t/r = 4.0 t/r =.0 t/r = 1.0 analytical numerical Radius r [mm] Figure 8: Convergence Study of ThroughThickness Compression Evidently, the numerical results converge to a final deflection with increasing ratio t/r. Although, it is found that even for a solid with t/r = 8, this deflection is still lower than w c(r). The reason for this difference in deformation can be found in the origin of w c(r). Sneddon [16] investigated the extension of a pennyshaped crack in an infinite solid, stressed with an internal pressure. Consequently, the occurring deformations are not affected by any constraints and the possible influence of a varying thickness t is not considered in the final deflection term, as per Equation (19). Nevertheless, to demonstrate the effectivity of w c(r) for an infinite solid, the same axisymmetric structure and procedure are applied as introduced above, however, to exclude any constraints due to boundary conditions not only a high thickness of t = 80 mm is applied, but the radial dimension of the solid is also extended to 0 mm. Further, only one 9
12 half of the bottom edge is pressurised, where the other half is fixed in throughthickness zdirection. The structure is illustrated in Figure 9 showing the vertical displacement in a contourplot. Figure 9: FEA of Pennyshaped Crack Model: System, Loading, Boundary Conditions and Distribution of w(r) In this case both approaches yield identical deflection curves, as per Figure 10. The outcome of this is that a consideration of throughthickness compression in terms of [16] can only be used as a first approximation, provided the applied repair thickness is sufficiently thick. Otherwise the portion of this component is significantly overestimated within the analytical model. 5. Conclusion The analytical and numerical investigation of a pressurised blister formation has highlighted several inaccuracies implemented in the ISOCode [10]. Hence, a parabolic distribution of the transverse shear stress τ rz is disregarded in the code s approach which leads to an overestimation of transverse shear effects. Although, it is a conservative assumption it is contradictory to an economic design of the FRP repair. Further, by the incorrect use of inplane elastic constants, the theoretical effects of throughthickness compression can be underestimated. As abovementioned, an underestimation of blister volume leads to an overestimation of the critical pressure p crit and is thus not acceptable. A comparison of the analytical and the numerical model has shown that the theoretically derived deflection terms for bending and transverse shear work accurately, provided a sufficiently small ratio of plate thickness t to plate radius R. On the contrary, it is found that a consideration of throughthickness compression is only justifiable for t/r > 0.5, i.e. when the effects of bending and shear deformation can be neglected due to the compact geometry of the structure. Further, it is stated that even for thick repairs the application of the approach after [16] can only be used as a first approximation. Hence, it is recommended to introduce a reduction factor considering decreasing compression due to decreasing thickness. Finally, it still needs to be clarified whether the idea of reducing the problem to the one of a clamped circular plate is possibly underestimating the problem, i.e. the volume of the blister. According to this, it is expected that especially 10
13 Deflection w c (r) [mm] analytical numerical Radius r [mm] Figure 10: Deflection of PennyShaped Crack Model in case of thin repairs the compliance of the surrounding repair material, with r > R, leads to a higher volumetric deflection. Due to the high complexity in deducing an analytical approach for a plate based on a compliant support, several FEA of different models have to be investigated to assess these effects and to determine possible increase factors. Acknowledgments This work was performed within the project Structure Repair and Rehabilitation of the Cooperative Research Centre for Advanced Composite Structures (CRCACS) Ltd in Melbourne, Australia. The lead author would like to acknowledge and thank CRCACS, particularly Professor Murray Scott and David Elder, for their invaluable assistance, support and guidance throughout this research. The author is also grateful for the financial support provided by the German Academic Exchange Service (DAAD). References [1] Batisse R. Review of gas transmission pipeline repair methods. In: Safety, Reliability and Risks Associated with Water, Oil and Gas Pipelines. NATO Science for Peace and Security Series C: Environmental Security; Springer Netherlands; 008, p [] Baker A. Bonded composite repair of fatiguecracked primary aircraft structure. Composite Structures 1999;47: [3] Tavakkolizadeh M, Saadatmanesh H. Strengthening of steelconcrete composite girders using carbon fiber reinforced polymers sheets. Journal of Structural Engineering 003;19: [4] Buyukozturk O, Hearing B. Failure behavior of precracked concrete beams retrofitted with FRP. Journal of Composites for Construction 1998;: [5] Duell JM, Wilson JM, Kessler MR. Analysis of a carbon composite overwrap pipeline repair system. International Journal of Pressure Vessels and Piping 008;85:78 8. [6] Goertzen WK, Kessler MR. Dynamic mechanical analysis of carbon/epoxy composites for structural pipeline repair. Composites Part B: Engineering 007;38:1 9. [7] Wagner W, Balzani C. Simulation of delamination in stringer stiffened fiberreinforced composite shells. Computers & Structures 008;86: [8] Balzani C, Wagner W. An interface element for the simulation of delamination in unidirectional fiberreinforced composite laminates. Engineering Fracture Mechanics 008;75: [9] Mableson AR, Dunn KR, Dodds N, Gibson AG. Refurbishment of steel tubular pipes using composite materials. Plastics, Rubber and Composites 000;9: [10] ISO/TS 4817:006: Petroleum, petrochemical and natural gas industries  composite repairs for pipework  qualification and design, installation, testing and inspection. Standard; International Organization for Standardization, Geneva, Switzerland; 006. [11] Griffith AA. The phenomena of rupture and flow in solids. Philosophical Transactions of the Royal Society of London 191;1: [1] Wang CH. Introduction to fracture mechanics. General document DSTOGD0103; Defence Sience and Technology Organisation; [13] Gross D, Seelig T. Linear fracture mechanics. In: Fracture Mechanics. Mechanical Engineering Series; Springer Berlin Heidelberg; 011, p [14] Timoshenko S, WoinowskyKrieger S. Theory of plates and shells. Engineering Societies Monographs; McGrawHill; [15] Panc V. Theories of elastic plates. Mechanics of Surface Structures Series; Noordhoff International Pub.;
14 [16] Sneddon IN. The distribution of stress in the neighbourhood of a crack in an elastic solid. Proceedings of the Royal Society of London Series A Mathematical and Physical Sciences 1946;187:9 60. [17] Harding JW, Sneddon IN. The elastic stresses produced by the indentation of the plane surface of a semiinfinite elastic solid by a rigid punch. Mathematical Proceedings of the Cambridge Philosophical Society 1945;41:16 6. [18] Key PL. A relation between crack surface displacements and the strain energy release rate. International Journal of Fracture 1969;5: [19] Gibson RF. Principles of composite material mechanics. Mechanical Engineering Series; CRC Press;. ed.; 007. [0] Taylor RL. FEAP a finite element analysis program. Theory manual version 8.3; Department of Civil and Environmental Engineering, University of California at Berkeley; 011. URL 1
USE OF CFRP LAMINATES FOR STRENGTHENING OF REINFORCED CONCRETE CORBELS
International Journal of Civil Engineering and Technology (IJCIET) Volume 6, Issue 11, Nov 2015, pp. 1120, Article ID: IJCIET_06_11_002 Available online at http://www.iaeme.com/ijciet/issues.asp?jtype=ijciet&vtype=6&itype=11
More informationComposite Design Fundamentals. David Richardson
Composite Design Fundamentals David Richardson Contents A review of the fundamental characteristics of composites Stiffness and Strength Anisotropic Role of fibre, matrix and interface Composite failure
More informationThe Fundamental Principles of Composite Material Stiffness Predictions. David Richardson
The Fundamental Principles of Composite Material Stiffness Predictions David Richardson Contents Description of example material for analysis Prediction of Stiffness using Rule of Mixtures (ROM) ROM with
More informationSEISMIC UPGRADE OF OAK STREET BRIDGE WITH GFRP
13 th World Conference on Earthquake Engineering Vancouver, B.C., Canada August 16, 2004 Paper No. 3279 SEISMIC UPGRADE OF OAK STREET BRIDGE WITH GFRP Yuming DING 1, Bruce HAMERSLEY 2 SUMMARY Vancouver
More informationShell Elements in ABAQUS/Explicit
ABAQUS/Explicit: Advanced Topics Appendix 2 Shell Elements in ABAQUS/Explicit ABAQUS/Explicit: Advanced Topics A2.2 Overview ABAQUS/Explicit: Advanced Topics ABAQUS/Explicit: Advanced Topics A2.4 Triangular
More informationGriffith theory of brittle fracture:
Griffith theory of brittle fracture: Observed fracture strength is always lower than theoretical cohesive strength. Griffith explained that the discrepancy is due to the inherent defects in brittle materials
More informationBending, Forming and Flexing Printed Circuits
Bending, Forming and Flexing Printed Circuits John Coonrod Rogers Corporation Introduction: In the printed circuit board industry there are generally two main types of circuit boards; there are rigid printed
More informationChapter 5 Bridge Deck Slabs. Bridge Engineering 1
Chapter 5 Bridge Deck Slabs Bridge Engineering 1 Basic types of bridge decks Insitu reinforced concrete deck (most common type) Precast concrete deck (minimize the use of local labor) Open steel grid
More informationFinite Element Formulation for Plates  Handout 3 
Finite Element Formulation for Plates  Handout 3  Dr Fehmi Cirak (fc286@) Completed Version Definitions A plate is a three dimensional solid body with one of the plate dimensions much smaller than the
More informationFailure, Analysis and Design. 2003, P. Joyce
Failure, nalysis and esign 23, P. Joyce Special Cases of Laminates The symmetry or antisymmetry of a laminate, based on angle, material, and thickness of plies, may zero out some elements of the three
More informationStructural Integrity Analysis
Structural Integrity Analysis 1. STRESS CONCENTRATION Igor Kokcharov 1.1 STRESSES AND CONCENTRATORS 1.1.1 Stress An applied external force F causes inner forces in the carrying structure. Inner forces
More informationSEISMIC RETROFITTING TECHNIQUE USING CARBON FIBERS FOR REINFORCED CONCRETE BUILDINGS
Fracture Mechanics of Concrete Structures Proceedings FRAMCOS3 AEDIFICA TIO Publishers, D79104 Freiburg, Germany SEISMIC RETROFITTING TECHNIQUE USING CARBON FIBERS FOR REINFORCED CONCRETE BUILDINGS H.
More informationCOMPUTATIONAL ENGINEERING OF FINITE ELEMENT MODELLING FOR AUTOMOTIVE APPLICATION USING ABAQUS
International Journal of Advanced Research in Engineering and Technology (IJARET) Volume 7, Issue 2, MarchApril 2016, pp. 30 52, Article ID: IJARET_07_02_004 Available online at http://www.iaeme.com/ijaret/issues.asp?jtype=ijaret&vtype=7&itype=2
More informationSimple design method
method Aim of the design method 2 3 Content of presentation in a fire situation method of reinforced concrete slabs at 20 C Floor slab model Failure modes method of at Extension to fire behaviour Membrane
More informationPrestressed Concrete Pipe Fitness for Service and Repair
Prestressed Concrete Pipe Fitness for Service and Repair Rasko Ojdrovic rpojdrovic@sgh.com 7819079231 IAEA  EPRI 15 October 2014 www.sgh.com SGH Pipeline Experience More than 25 years of research, analysis,
More informationMECHANICS OF SOLIDS  BEAMS TUTORIAL 1 STRESSES IN BEAMS DUE TO BENDING. On completion of this tutorial you should be able to do the following.
MECHANICS OF SOLIDS  BEAMS TUTOIAL 1 STESSES IN BEAMS DUE TO BENDING This is the first tutorial on bending of beams designed for anyone wishing to study it at a fairly advanced level. You should judge
More informationTorsion Tests. Subjects of interest
Chapter 10 Torsion Tests Subjects of interest Introduction/Objectives Mechanical properties in torsion Torsional stresses for large plastic strains Type of torsion failures Torsion test vs.tension test
More informationPunching shear behavior of steelconcrete composite decks with different shear connectors
Punching shear behavior of steelconcrete composite decks with different shear connectors *XiaoQing Xu 1) and YuQing Liu 2) 1), 2) Department of Bridge Engineering, Tongji University, Shanghai 200092,
More informationOptimum proportions for the design of suspension bridge
Journal of Civil Engineering (IEB), 34 (1) (26) 114 Optimum proportions for the design of suspension bridge Tanvir Manzur and Alamgir Habib Department of Civil Engineering Bangladesh University of Engineering
More informationCourse in. Nonlinear FEM
Course in Introduction Outline Lecture 1 Introduction Lecture 2 Geometric nonlinearity Lecture 3 Material nonlinearity Lecture 4 Material nonlinearity continued Lecture 5 Geometric nonlinearity revisited
More informationNumerical Analysis of Independent Wire Strand Core (IWSC) Wire Rope
Numerical Analysis of Independent Wire Strand Core (IWSC) Wire Rope Rakesh Sidharthan 1 Gnanavel B K 2 Assistant professor Mechanical, Department Professor, Mechanical Department, Gojan engineering college,
More informationThe Original Carbon Fiber Reinforced Polymer System
Infrastructure The Original Carbon Fiber Reinforced Polymer System Phone: 52.292.39 Toll Free: 866.38.269 Fax: 52.48.5274 282 E. Fort Lowell Rd. Tucson, AZ 8576 www.dowaksausa.com Test results are supported
More informationBehaviour of retrofitted reinforced concrete beams under combined bending and torsion : A numerical study
Behaviour of retrofitted reinforced concrete beams under combined bending and torsion : A numerical study R.Santhakumar Assistant Professor, National Institute of Technical Teachers Training and Research,
More informationInsitu Load Testing to Evaluate New Repair Techniques
Insitu Load Testing to Evaluate New Repair Techniques W.J. Gold 1 and A. Nanni 2 1 Assistant Research Engineer, Univ. of Missouri Rolla, Dept. of Civil Engineering 2 V&M Jones Professor, Univ. of Missouri
More informationFatigue. Figure 41 Typical Comparison of Metal and Composite Fatigue Damage [Salkind, Fatigue of Composites]
Chapter Four PERFORMANCE Fatigue A fundamental problem concerning the engineering uses of fiber reinforced plastics (FRP) is the determination of their resistance to combined states of cyclic stress. [41]
More informationFLEXURAL PERFORMANCE OF RC BEAMS STRENGTHENED WITH PRESTRESSED CFRP SHEETS
FLEXURAL PERFORMANCE OF RC BEAMS STRENGTHENED WITH PRESTRESSED CFRP SHEETS Piyong Yu, Pedro F. Silva, Antonio Nanni Center for Infrastructure and Engineering Studies Department of Civil, Architectural,
More informationANALYTICAL AND EXPERIMENTAL EVALUATION OF SPRING BACK EFFECTS IN A TYPICAL COLD ROLLED SHEET
International Journal of Mechanical Engineering and Technology (IJMET) Volume 7, Issue 1, JanFeb 2016, pp. 119130, Article ID: IJMET_07_01_013 Available online at http://www.iaeme.com/ijmet/issues.asp?jtype=ijmet&vtype=7&itype=1
More informationEFFECTS ON NUMBER OF CABLES FOR MODAL ANALYSIS OF CABLESTAYED BRIDGES
EFFECTS ON NUMBER OF CABLES FOR MODAL ANALYSIS OF CABLESTAYED BRIDGES YangCheng Wang Associate Professor & Chairman Department of Civil Engineering Chinese Military Academy FengShan 83000,Taiwan Republic
More informationMETHODS FOR ACHIEVEMENT UNIFORM STRESSES DISTRIBUTION UNDER THE FOUNDATION
International Journal of Civil Engineering and Technology (IJCIET) Volume 7, Issue 2, MarchApril 2016, pp. 4566, Article ID: IJCIET_07_02_004 Available online at http://www.iaeme.com/ijciet/issues.asp?jtype=ijciet&vtype=7&itype=2
More informationNonlinear Models of Reinforced and Posttensioned Concrete Beams
111 Nonlinear Models of Reinforced and Posttensioned Concrete Beams ABSTRACT P. Fanning Lecturer, Department of Civil Engineering, University College Dublin Earlsfort Terrace, Dublin 2, Ireland. Email:
More informationStructural Failures Cost Lives and Time
Structural Failures Cost Lives and Time Recent failures of storage bins, silos and other structures highlight the need to increase awareness of hazards associated with these structures. Since 2010, one
More informationDesigner s NOTEBOOK BLAST CONSIDERATIONS
Designer s NOTEBOOK BLAST CONSIDERATIONS For a surface blast, the most directly affected building elements are the façade and structural members on the lower four stories. Although the walls can be designed
More informationMATERIALS AND SCIENCE IN SPORTS. Edited by: EH. (Sam) Froes and S.J. Haake. Dynamics
MATERIALS AND SCIENCE IN SPORTS Edited by: EH. (Sam) Froes and S.J. Haake Dynamics Analysis of the Characteristics of Fishing Rods Based on the LargeDeformation Theory Atsumi Ohtsuki, Prof, Ph.D. Pgs.
More informationA NOVEL STRENGTH MODEL FOR UNIDIRECTIONAL FIBRE REINFORCED COMPOSITES WITH REALISTIC FIBRE PACKINGS
THE 19 TH INTERNATIONAL CONFERENCE ON COMPOSITE MATERIALS A NOVEL STRENGTH MODEL FOR UNIDIRECTIONAL FIBRE REINFORCED COMPOSITES WITH REALISTIC FIBRE PACKINGS Y. Swolfs 1, L. Gorbatikh 1, I. Verpoest*
More informationTensile fracture analysis of blunt notched PMMA specimens by means of the Strain Energy Density
Engineering Solid Mechanics 3 (2015) 3542 Contents lists available at GrowingScience Engineering Solid Mechanics homepage: www.growingscience.com/esm Tensile fracture analysis of blunt notched PMMA specimens
More informationNew approaches in Eurocode 3 efficient global structural design
New approaches in Eurocode 3 efficient global structural design Part 1: 3D model based analysis using general beamcolumn FEM Ferenc Papp* and József Szalai ** * Associate Professor, Department of Structural
More informationAn Overview of the Finite Element Analysis
CHAPTER 1 An Overview of the Finite Element Analysis 1.1 Introduction Finite element analysis (FEA) involves solution of engineering problems using computers. Engineering structures that have complex geometry
More informationLOADCARRYING CAPACITY OF AXIALLY LOADED RODS GLUEDIN PERPENDICULAR TO THE GRAIN
LOADCARRYING CAPACITY OF AXIALLY LOADED RODS GLUEDIN PERPENDICULAR TO TE GRAIN Prof. Dr.Ing..J. Blaß, Dipl.Ing. B. Laskewitz Universität Karlsruhe (T), Germany Abstract Gluedin rods have been used
More informationDeflection Calculation of RC Beams: Finite Element Software Versus Design Code Methods
Deflection Calculation of RC Beams: Finite Element Software Versus Design Code Methods G. Kaklauskas, Vilnius Gediminas Technical University, 1223 Vilnius, Lithuania (gintaris.kaklauskas@st.vtu.lt) V.
More informationEXPERIMENTAL AND NUMERICAL ANALYSIS OF THE COLLAR PRODUCTION ON THE PIERCED FLAT SHEET METAL USING LASER FORMING PROCESS
JOURNAL OF CURRENT RESEARCH IN SCIENCE (ISSN 23225009) CODEN (USA): JCRSDJ 2014, Vol. 2, No. 2, pp:277284 Available at www.jcrs010.com ORIGINAL ARTICLE EXPERIMENTAL AND NUMERICAL ANALYSIS OF THE COLLAR
More informationOptimising plate girder design
Optimising plate girder design NSCC29 R. Abspoel 1 1 Division of structural engineering, Delft University of Technology, Delft, The Netherlands ABSTRACT: In the design of steel plate girders a high degree
More informationSTRESS AND DEFORMATION ANALYSIS OF LINEAR ELASTIC BARS IN TENSION
Chapter 11 STRESS AND DEFORMATION ANALYSIS OF LINEAR ELASTIC BARS IN TENSION Figure 11.1: In Chapter10, the equilibrium, kinematic and constitutive equations for a general threedimensional solid deformable
More informationCAD and Finite Element Analysis
CAD and Finite Element Analysis Most ME CAD applications require a FEA in one or more areas: Stress Analysis Thermal Analysis Structural Dynamics Computational Fluid Dynamics (CFD) Electromagnetics Analysis...
More informationField Damage Inspection and Static Load Test Analysis of Jiamusi Highway Prestressed Concrete Bridge in China
Advanced Materials Research Vols. 163167 (2011) pp 11471156 Online available since 2010/Dec/06 at www.scientific.net (2011) Trans Tech Publications, Switzerland doi:10.4028/www.scientific.net/amr.163167.1147
More informationMATERIALS SELECTION FOR SPECIFIC USE
MATERIALS SELECTION FOR SPECIFIC USE1 Subtopics 1 Density What determines density and stiffness? Material properties chart Design problems LOADING 2 STRENGTH AND STIFFNESS Stress is applied to a material
More informationPOLITECNICO DI TORINO. Engineering Faculty Master s Degree in Aerospace Engineering. Final Thesis
POLITECNICO DI TORINO Engineering Faculty Master s Degree in Aerospace Engineering Final Thesis DETECTION AND ANALYSIS OF BARELY VISIBLE IMPACT DAMAGE AND ITS PROGRESSION ON A COMPOSITE OVERWRAPPED PRESSURE
More informationStructural model of closed circular cylindrical shell for polutionfree transportation of materials.
University of Wollongong Research Online Wollongong University College Bulletin Corporate Publications Archive 1972 Structural model of closed circular cylindrical shell for polutionfree transportation
More informationCarbon Fiber Reinforced Polymer (CFRP) as Reinforcement for Concrete Beam
Carbon Fiber Reinforced Polymer (CFRP) as Reinforcement for Concrete Beam Norazman Mohamad Nor 1, Mohd Hanif Ahmad Boestamam, Mohammed Alias Yusof 3 1,3 Universiti Pertahanan Nasional Malaysia, 57000 Kuala
More informationANALYSIS FOR BEHAVIOR AND ULTIMATE STRENGTH OF CONCRETE CORBELS WITH HYBRID REINFORCEMENT
International Journal of Civil Engineering and Technology (IJCIET) Volume 6, Issue 10, Oct 2015, pp. 2535 Article ID: IJCIET_06_10_003 Available online at http://www.iaeme.com/ijciet/issues.asp?jtype=ijciet&vtype=6&itype=10
More informationCHAPTER 1 INTRODUCTION
CHAPTER 1 INTRODUCTION 1.1 Background of the research Beam is a main element in structural system. It is horizontal member that carries load through bending (flexure) action. Therefore, beam will deflect
More informationENGI 8673 Subsea Pipeline Engineering Faculty of Engineering and Applied Science
GUIDANCE NOTE LECTURE 12 THERMAL EXPANSION ANALYSIS OVERVIEW The calculation procedure for determining the longitudinal pipeline response can be formulated on the basis of strain. The longitudinal strain
More informationCARBON/DYNEEMA INTRALAMINAR HYBRIDS: NEW STRATEGY TO INCREASE IMPACT RESISTANCE OR DECREASE MASS OF CARBON FIBER COMPOSITES
26 TH INTERNATIONAL CONGRESS OF THE AERONAUTICAL SCIENCES CARBON/DYNEEMA INTRALAMINAR HYBRIDS: NEW STRATEGY TO INCREASE IMPACT RESISTANCE OR DECREASE MASS OF CARBON FIBER COMPOSITES J. G. H. Bouwmeester*,
More informationTechnology of EHIS (stamping) applied to the automotive parts production
Laboratory of Applied Mathematics and Mechanics Technology of EHIS (stamping) applied to the automotive parts production Churilova Maria, SaintPetersburg State Polytechnical University Department of Applied
More informationTHE DETERMINATION OF DELAMINATION STRAIN ENERGY RELEASE RATE OF COMPOSITE BIMATERIAL INTERFACE
THE DETERMINATION OF DELAMINATION STRAIN ENERGY RELEASE RATE OF COMPOSITE BIMATERIAL INTERFACE Jaroslav Juracka, Vladimir Matejak Brno University of Technology, Institute of Aerospace Engineering juracka@fme.vutbr.cz;
More informationEXPERIMENTAL EVALUATION OF REINFORCED CONCRETE BEAM RETROFITTED WITH FERROCEMENT
Int. J. Struct. & Civil Engg. Res. 2013 Y V Ladi and P M Mohite, 2013 Research Paper EXPERIMENTAL EVALUATION OF REINFORCED CONCRETE BEAM RETROFITTED WITH FERROCEMENT Y V Ladi 1 * and P M Mohite 2 *Corresponding
More informationTechnical Report Example (1) Chartered (CEng) Membership
Technical Report Example (1) Chartered (CEng) Membership A TECHNICAL REPORT IN SUPPORT OF APPLICATION FOR CHARTERED MEMBERSHIP OF IGEM DESIGN OF 600 (103 BAR) 820MM SELF SEALING REPAIR CLAMP AND VERIFICATION
More information8.2 Elastic Strain Energy
Section 8. 8. Elastic Strain Energy The strain energy stored in an elastic material upon deformation is calculated below for a number of different geometries and loading conditions. These expressions for
More informationFAILURE MODES and MATERIALS PROPERTIES. Component failures. Ductile and Brittle Fracture COMPONENT FAILURES. COMPONENT FAILURE MODES examples:
FAILURE MODES and MATERIALS PROPERTIES MECH2300  Materials Lecture 10 R. W. Truss Materials Engineering R.Truss@uq.edu.au COMPONENT FAILURES Structures lectures es on component es cause response in component
More informationSection 16: Neutral Axis and Parallel Axis Theorem 161
Section 16: Neutral Axis and Parallel Axis Theorem 161 Geometry of deformation We will consider the deformation of an ideal, isotropic prismatic beam the cross section is symmetric about yaxis All parts
More informationNumerical modelling of shear connection between concrete slab and sheeting deck
7th fib International PhD Symposium in Civil Engineering 2008 September 1013, Universität Stuttgart, Germany Numerical modelling of shear connection between concrete slab and sheeting deck Noémi Seres
More informationCFRP STRENGTHENING OF CIRCULAR CONCRETE SLAB WITH AND WITHOUT OPENINGS
International Journal of Civil Engineering and Technology (IJCIET) Volume 7, Issue 1, JanFeb 2016, pp. 290303, Article ID: IJCIET_07_01_024 Available online at http://www.iaeme.com/ijciet/issues.asp?jtype=ijciet&vtype=7&itype=1
More informationEML 5526 FEA Project 1 Alexander, Dylan. Project 1 Finite Element Analysis and Design of a Plane Truss
Problem Statement: Project 1 Finite Element Analysis and Design of a Plane Truss The plane truss in Figure 1 is analyzed using finite element analysis (FEA) for three load cases: A) Axial load: 10,000
More informationIMPROVING THE STRUT AND TIE METHOD BY INCLUDING THE CONCRETE SOFTENING EFFECT
International Journal of Civil Engineering and Technology (IJCIET) Volume 7, Issue 2, MarchApril 2016, pp. 117 127, Article ID: IJCIET_07_02_009 Available online at http://www.iaeme.com/ijciet/issues.asp?jtype=ijciet&vtype=7&itype=2
More informationTHERMAL CRACKING RESPONE OF REINFORCED CONCRETE BEAM TO GRADIENT TEMPERATURE
THERMAL CRACKING RESPONE OF REINFORCED CONCRETE BEAM TO GRADIENT TEMPERATURE L. DAHMANI, M.KOUANE Abstract In this paper are illustrated the principal aspects connected with the numerical evaluation of
More informationTechnical Notes 3B  Brick Masonry Section Properties May 1993
Technical Notes 3B  Brick Masonry Section Properties May 1993 Abstract: This Technical Notes is a design aid for the Building Code Requirements for Masonry Structures (ACI 530/ASCE 5/TMS 40292) and Specifications
More informationFinite Element Formulation for Beams  Handout 2 
Finite Element Formulation for Beams  Handout 2  Dr Fehmi Cirak (fc286@) Completed Version Review of EulerBernoulli Beam Physical beam model midline Beam domain in threedimensions Midline, also called
More informationDifferential Relations for Fluid Flow. Acceleration field of a fluid. The differential equation of mass conservation
Differential Relations for Fluid Flow In this approach, we apply our four basic conservation laws to an infinitesimally small control volume. The differential approach provides point by point details of
More informationCarbon Fiber Reinforced Polymer (CFRP) Laminates  Aslan
Carbon Fiber Reinforced Polymer (CFRP) Laminates  Aslan 400 series November 10, 2011 Aslan 400 Carbon FRP Laminates are used to structurally strengthen existing concrete, wood, or masonry members in flexure
More informationSHARP EDGE EFFECTS ON FRP CONFINEMENT OF RC SQUARE COLUMNS. Abstract. Introduction
SHARP EGE EFFECTS ON FRP CONFINEMENT OF RC SQUARE COLUMNS Raquel Fernandes de Paula, Univ. Nova de Lisboa, PORTUGAL Manuel Gonçalves da Silva, Univ. Nova de Lisboa, PORTUGAL Abstract Shape of cross sections
More informationPlates and Shells: Theory and Computation  4D9  Dr Fehmi Cirak (fc286@) Office: Inglis building mezzanine level (INO 31)
Plates and Shells: Theory and Computation  4D9  Dr Fehmi Cirak (fc286@) Office: Inglis building mezzanine level (INO 31) Outline 1! This part of the module consists of seven lectures and will focus
More informationThe elements used in commercial codes can be classified in two basic categories:
CHAPTER 3 Truss Element 3.1 Introduction The single most important concept in understanding FEA, is the basic understanding of various finite elements that we employ in an analysis. Elements are used for
More informationUse of Strain Gauge Rosette to Investigate Stress concentration in Isotropic and Orthotropic Plate with Circular Hole
Use of Strain Gauge Rosette to Investigate Stress concentration in Isotropic and Orthotropic Plate with Circular Hole Mr.V.G.Aradhye 1, Prof.S.S.Kulkarni 2 1 PG Scholar, Mechanical department, SKN Sinhgad
More informationStresses in Beam (Basic Topics)
Chapter 5 Stresses in Beam (Basic Topics) 5.1 Introduction Beam : loads acting transversely to the longitudinal axis the loads create shear forces and bending moments, stresses and strains due to V and
More informationgéopolymère GEOPOLYMER for Repair and Rehabilitation of Reinforced concrete beams
géopolymère GEOPOLYMER for Repair and Rehabilitation of Reinforced concrete beams Project GEOSTRUCTURE FireProof External repair and structural retrofit for aging infrastructure, aging buildings, earthquake
More informationLap Fillet Weld Calculations and FEA Techniques
Lap Fillet Weld Calculations and FEA Techniques By: MS.ME Ahmad A. Abbas Sr. Analysis Engineer Ahmad.Abbas@AdvancedCAE.com www.advancedcae.com Sunday, July 11, 2010 Advanced CAE All contents Copyright
More informationMETU DEPARTMENT OF METALLURGICAL AND MATERIALS ENGINEERING
METU DEPARTMENT OF METALLURGICAL AND MATERIALS ENGINEERING Met E 206 MATERIALS LABORATORY EXPERIMENT 1 Prof. Dr. Rıza GÜRBÜZ Res. Assist. Gül ÇEVİK (Room: B306) INTRODUCTION TENSION TEST Mechanical testing
More informationDESIGN OF SLABS. 3) Based on support or boundary condition: Simply supported, Cantilever slab,
DESIGN OF SLABS Dr. G. P. Chandradhara Professor of Civil Engineering S. J. College of Engineering Mysore 1. GENERAL A slab is a flat two dimensional planar structural element having thickness small compared
More informationSTRENGTHENING STEELCONCRETE COMPOSITE GIRDERS USING FRPs: STATEOFTHEART
AsiaPacific Conference on FRP in Structures (APFIS 2007) S.T. Smith (ed) 2007 International Institute for FRP in Construction STRENGTHENING STEELCONCRETE COMPOSITE GIRDERS USING FRPs: STATEOFTHEART
More informationB.TECH. (AEROSPACE ENGINEERING) PROGRAMME (BTAE) TermEnd Examination December, 2011 BAS010 : MACHINE DESIGN
No. of Printed Pages : 7 BAS01.0 B.TECH. (AEROSPACE ENGINEERING) PROGRAMME (BTAE) CV CA CV C:) O TermEnd Examination December, 2011 BAS010 : MACHINE DESIGN Time : 3 hours Maximum Marks : 70 Note : (1)
More informationAPE T CFRP Aslan 500
Carbon Fiber Reinforced Polymer (CFRP) Tape is used for structural strengthening of concrete, masonry or timber elements using the technique known as Near Surface Mount or NSM strengthening. Use of CFRP
More informationThe Mathematics of Simple Beam Deflection
The Mathematics of Simple Beam Laing O Rourke Civil Engineering INTRODUCTION Laing O Rourke plc is the largest privately owned construction firm in the UK. It has offices in the UK, Germany, India, Australia
More informationCH 6: Fatigue Failure Resulting from Variable Loading
CH 6: Fatigue Failure Resulting from Variable Loading Some machine elements are subjected to static loads and for such elements static failure theories are used to predict failure (yielding or fracture).
More information(Seattle is home of Boeing Jets)
Dr. Faeq M. Shaikh Seattle, Washington, USA (Seattle is home of Boeing Jets) 1 Pre Requisites for Today s Seminar Basic understanding of Finite Element Analysis Working Knowledge of Laminate Plate Theory
More informationBEHAVIOR OF SHORT CONCRETE COLUMNS REINFORCED BY CFRP BARS AND SUBJECTED TO ECCENTRIC LOAD
International Journal of Civil Engineering and Technology (IJCIET) Volume 6, Issue 10, Oct 2015, pp. 1524 Article ID: IJCIET_06_10_002 Available online at http://www.iaeme.com/ijciet/issues.asp?jtype=ijciet&vtype=6&itype=10
More informationModule 3. Limit State of Collapse  Flexure (Theories and Examples) Version 2 CE IIT, Kharagpur
Module 3 Limit State of Collapse  Flexure (Theories and Examples) Lesson 4 Computation of Parameters of Governing Equations Instructional Objectives: At the end of this lesson, the student should be able
More informationStress Strain Relationships
Stress Strain Relationships Tensile Testing One basic ingredient in the study of the mechanics of deformable bodies is the resistive properties of materials. These properties relate the stresses to the
More informationInternational Journal of Engineering ResearchOnline A Peer Reviewed International Journal Articles available online http://www.ijoer.
RESEARCH ARTICLE ISSN: 23217758 DESIGN AND DEVELOPMENT OF A DYNAMOMETER FOR MEASURING THRUST AND TORQUE IN DRILLING APPLICATION SREEJITH C 1,MANU RAJ K R 2 1 PG Scholar, M.Tech Machine Design, Nehru College
More informationDesign of Steel Structures Prof. S.R.Satish Kumar and Prof. A.R.Santha Kumar
6.3 Behaviour of steel beams Laterally stable steel beams can fail only by (a) Flexure (b) Shear or (c) Bearing, assuming the local buckling of slender components does not occur. These three conditions
More informationAdhesion and Viscoelasticity Properties of PVB in Laminated Safety Glass
Adhesion and Viscoelasticity Properties of PVB in Laminated Safety Glass Maurizio FROLI Professor Department of Civil Engineering, Structural Division University of Pisa, Pisa, Italy Maurizio Froli, born
More informationDesign of crossgirders and slabs in ladder deck bridges
130 Chris R Hendy Head of Bridge Design and Technology Highways & Transportation Atkins Jessica Sandberg Senior Engineer Highways & Transportation Atkins David Iles Steel Construction Institute Design
More informationDesign of Carbon Composite Driveshaft for Ultralight Aircraft Propulsion System R. Poul, P. Růžička,. D. Hanus, K. Blahouš
Design of Carbon Composite Driveshaft for Ultralight Aircraft Propulsion System R. Poul, P. Růžička,. D. Hanus, K. Blahouš This paper deals with the design of the carbon fibre composite driveshaft. This
More informationAnalysis of Reinforced Concrete Beams Strengthened with Composites. Subjected to Fatigue Loading
Analysis of Reinforced Concrete Beams Strengthened with Composites Subjected to Fatigue Loading By Christos G. Papakonstantinou, Perumalsamy. Balaguru and Michael F. Petrou Synopsis: Use of high strength
More informationStress and Deformation Analysis. Representing Stresses on a Stress Element. Representing Stresses on a Stress Element con t
Stress and Deformation Analysis Material in this lecture was taken from chapter 3 of Representing Stresses on a Stress Element One main goals of stress analysis is to determine the point within a loadcarrying
More informationMUKAVEMET KIRILMA HİPOTEZLERİ
1 MUKAVEMET KIRILMA HİPOTEZLERİ 17. Theories of failure or yield criteria (1) Maximum shearing stress theory (2) Octahedral shearing stress theory (3) Maximum normal stress theory for brittle materials.
More informationUnit 6 Plane Stress and Plane Strain
Unit 6 Plane Stress and Plane Strain Readings: T & G 8, 9, 10, 11, 12, 14, 15, 16 Paul A. Lagace, Ph.D. Professor of Aeronautics & Astronautics and Engineering Systems There are many structural configurations
More informationSEISMIC RETROFITTING OF STRUCTURES
SEISMIC RETROFITTING OF STRUCTURES RANJITH DISSANAYAKE DEPT. OF CIVIL ENGINEERING, FACULTY OF ENGINEERING, UNIVERSITY OF PERADENIYA, SRI LANKA ABSTRACT Many existing reinforced concrete structures in present
More informationAN AD OPTIMIZED METHOD FOR THE STRUCTURAL ANALYSIS OF PRESSURE VESSELS
Proceedings of ICAD2014 ICAD201424 AN AD OPTIMIZED METHOD FOR THE STRUCTURAL ANALYSIS OF PRESSURE VESSELS ABSTRACT Andrea Girgenti a.girgenti@unimarconi.it Alessandro Giorgetti a.giorgetti@unimarconi.it
More informationSEISMIC DESIGN. Various building codes consider the following categories for the analysis and design for earthquake loading:
SEISMIC DESIGN Various building codes consider the following categories for the analysis and design for earthquake loading: 1. Seismic Performance Category (SPC), varies from A to E, depending on how the
More informationChapter Outline. Mechanical Properties of Metals How do metals respond to external loads?
Mechanical Properties of Metals How do metals respond to external loads? Stress and Strain Tension Compression Shear Torsion Elastic deformation Plastic Deformation Yield Strength Tensile Strength Ductility
More informationME111 Lecture 16 1. ME111 Instructor: Peter Pinsky Class #16 November 1, 2000
Toda s Topics ME111 Instructor: Peter Pinsk Class #16 November 1, 2000 Introduction to linear elastic fracture mechanics (LEFM). Problem 3 A centercracked plate of AII 1144 steel ( C = 115MPa m ) has
More information